Research Article www.acsami.org
Al2O3 on Black Phosphorus by Atomic Layer Deposition: An in Situ Interface Study Hui Zhu,† Stephen McDonnell,† Xiaoye Qin,† Angelica Azcatl,† Lanxia Cheng,† Raﬁk Addou,† Jiyoung Kim,† Peide D. Ye,‡ and Robert M. Wallace*,† †
Department of Materials Science and Engineering, University of Texas at Dallas, Richardson, Texas 75080, United States School of Electrical and Computer Engineering and Birck Nanotechnology Center, Purdue University, West Lafayette, Indiana 47907, United States
S Supporting Information *
ABSTRACT: In situ “half cycle” atomic layer deposition (ALD) of Al2O3 was carried out on black phosphorus (“blackP”) surfaces with modiﬁed phosphorus oxide concentrations. X-ray photoelectron spectroscopy is employed to investigate the interfacial chemistry and the nucleation of the Al2O3 on black-P surfaces. This work suggests that exposing a sample that is initially free of phosphorus oxide to the ALD precursors does not result in detectable oxidation. However, when the phosphorus oxide is formed on the surface prior to deposition, the black-P can react with both the surface adventitious oxygen contamination and the H2O precursor at a deposition temperature of 200 °C. As a result, the concentration of the phosphorus oxide increases after both annealing and the atomic layer deposition process. The nucleation rate of Al2O3 on black-P is correlated with the amount of oxygen on samples prior to the deposition. The growth of Al2O3 follows a “substrate inhibited growth” behavior where an incubation period is required. Ex situ atomic force microscopy is also used to investigate the deposited Al2O3 morphologies on black-P where the Al2O3 tends to form islands on the exfoliated black-P samples. Therefore, surface functionalization may be needed to get a conformal coverage of Al2O3 on the phosphorus oxide free samples. KEYWORDS: black phosphorus, surface oxidation, atomic layer deposition, aluminum oxide, water, X-ray photoelectron spectroscopy al.3 and Wood et al.13 mentioned that the Al2O3 passivated fewlayer black-P metal oxide semiconductor ﬁeld-eﬀect transistors (MOSFET) can be stable in air for more than 100 h. However, there are still many unsolved problems for high-k/black-P heterostructures such as lower ﬁeld mobilities (40−100 cm2/ (V·s)) with respect to BN/black-P/BN and trapped charge issues.2,3,13 It is still unclear whether surface oxidation by ambient conditions degenerates the electronic properties of ALD Al2O3/black-P. Toward this end, three diﬀerent samples oxidized by ambient air were investigated to understand the interfacial interaction, chemistry, and nucleation of atomic layer deposited Al2O3 on black-P using a combination of in situ monochromatic X-ray photoelectron spectroscopy (XPS) and ex situ atomic force microscopy (AFM).
1. INTRODUCTION Black phosphorus (“black-P”) is an anisotropic lamellar semiconductor considered to be an appealing two-dimensional (2D) material because of its novel properties and potential application in few-layer transistor structures.1−7 Bulk black-P has a direct bandgap of about 0.3 eV,2,8,9 and an impressive hole mobility of up to 104 cm2/(V·s) at low temperatures (50−100 K).10,11 Few-layer black-P ﬁeld eﬀect transistors possess high current on/oﬀ ratios (up to 104) and high carrier mobilities up to 1000 cm2/(V·s) at room temperature.1,2 Consequently, black-P is a promising candidate for nanoelectronic and optoelectronic device applications.12 However, a clear challenge in the implementation of black-P is the strong hydrophilic13,14 and oxidation9 reactions during device processing and thereafter. Thus, eﬃcient isolation/passivation layers are necessary for black-P to preserve its electronic properties. To date, many eﬀorts on passivation have been reported. For example, recent reports show that the high ﬁeld-eﬀect mobility (∼1350−4000 cm2/(V·s)) of a hexagonal boron nitride (h-BN) isolated BN/ black-P/BN heterostructure15−17 is stable in an atmospheric ambient for more than 1 week. Al2O32,3,18 or HfO219 dielectric layers deposited by atomic layer deposition (ALD) are also used as passivation layers in recent black-P transistors. Luo et © XXXX American Chemical Society
2. EXPERIMENTAL SECTION Three black-P samples (thickness ∼1 mm), synthesized and purchased from Smart Elements, were used in this study. One is examined “as received” with a native oxide (“S1”) present on the surface, and another two (“S2” and “S3”) were cleaned by mechanical exfoliation Received: April 13, 2015 Accepted: May 28, 2015
DOI: 10.1021/acsami.5b03192 ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXX
ACS Applied Materials & Interfaces with Scotch Magic tape, which removes the outer layers of the crystal before loading the samples in ultrahigh vacuum (UHV). The UHV system used in this work was described in detail elsewhere20 and connects a surface analysis chamber and a Picosun 200R ALD chamber (base pressure ∼4 mbar) through a UHV (∼10−10 mbar) transfer tube, preventing spurious surface contamination during the experiment. To control surface oxidation, the S2 sample was oxidized by ambient air exposure for 5 min, whereas the S3 sample was loaded into the UHV chamber immediately after exfoliation (less than 2 min ambient exposure). In this experiment, ALD of Al2O3 was carried out with successive cycles of trimethylaluminum (TMA) and H2O precursors, with an argon (Ar) carrier gas (99.9997%, Airgas) at a ﬂow rate of 200 sccm, 0.1 s pulse + 4 s Ar purge time for TMA, 0.1 s pulse + 6 s Ar purge time for H2O at a substrate temperature of 200 °C. To monitor the Al2O3 growth on black phosphorus, the XPS scans were taken as follows: (i) on the initial surfaces, (ii) after exposing samples to the ALD vacuum ambient at 200 °C for 1 h, (iii) after each successive half cycle21 of TMA and H2O up to two full cycles, as well as after (iv) 5, 10, 20, 30, and 40 full cycles (TMA + H2O). Additional XPS scans were performed on the S3 sample after 60 and 80 full cycles. XPS spectra were taken of the P 2p, Al 2p, Sn 3d, I 3d, C 1s and O 1s, core level regions using a monochromatic Al Kα X-ray source (hν = 1486.7 eV) with a takeoﬀ angle of 45° from the substrate normal and a pass energy of 15 eV. The deconvolution of XPS was carried out with AAnalyzer software.22 The AFM images of the samples after 40 cycles of Al2O3 were recorded on three samples using an ex situ Veeco (Bruker) multimode system in noncontact tapping mode. To compare the Al2O3 growth on the S1 and S3 samples, AFM images were also obtained on the S3 sample after 80 cycles of Al2O3, which has a comparable Al2O3 thickness to that of the S1 sample. The AFM images were analyzed using WSxM software.
below the XPS detection limit (∼0.1 at.%) for sample S3. In Figure 1b, integrated intensity ratio of the total phosphorus oxide (IP‑O) feature to the integrated intensity of the bulk blackP feature (IP‑P) is shown. The IP‑O/IP‑P ratios on the initial S1 and S2 samples are estimated to be 0.1 and 0.03, respectively. The phosphorus oxide thicknesses were estimated, using XPS peak attenuation (see the Supporting Information) for samples S1 and S2, to be ∼0.27 and ∼0.08 nm, respectively. To diﬀerentiate clearly between thermal eﬀects and surface reactions with ALD precursors, the three samples were exposed to the ALD reactor environment at 200 °C for 1 h under Ar ﬂow (P ∼4 mbar), and were subsequently analyzed by XPS without any ALD precursor exposure. After this process, a saturated phosphorus oxide chemical state (P2O5)24−26 is clearly detected at 135.1 ± 0.05 eV on the S1 sample. This feature is also observed with a lower intensity on the S2 sample. The intensity ratio IP‑O/IP‑P (seen in Figure 1b) after annealing increases to 0.2 and 0.05 on the S1 and S2 samples, respectively, while remaining below the XPS detection limit on the S3 sample. The estimated phosphorus oxide thicknesses after annealing are ∼0.33 and ∼0.13 nm for samples S1 and S2, respectively. In addition, the original POx peak (at 134.2 eV) does not decrease after annealing, suggesting that the formation of P2O5 originates from the adsorption of oxygen, not only the conversion from POx to P2O5 with temperature. Oxygen sources are likely the surface adventitious contamination such as O−C(H) species that are detectable on every sample (shown in the Supporting Information Figures S1 and S2). A similar phenomenon is also found in our previous ALD half cycle study of AlGaN, where the surface oxygen contamination results in the increase of Ga/Al−O concentration during the initial annealing prior to ALD.27−29 Recent density functional theory (DFT) calculations suggest that the most favorable sites for oxygen on black-P depends on the amount of oxygen being adsorbed.30 Considering the reaction of an oxygen atom24,30 or an O2 molecule30 with an ideal, defect free black-P surface, the direct adsorption of oxygen on top of a single P atom, with the underlying black-P structure remaining unchanged, is relatively more favorable than bridging between two P atoms for low oxygen concentrations, such as 2 oxygen atoms per unit cell), both direct adsorption on top of a single P atom and also bridge bonding between two P atoms are energetically favorable and result in the formation of planar or tubular phosphorus oxides such as P2O3 or P2O5.30 It should be noted that the lattice constants of some phosphorus oxides, such as tubular-P2O5, can be 1.9 times larger than that of black-P, leading to obvious black-P lattice deformation through bond scission and O insertion.30 Therefore, in samples S1 and S2, the higher concentration of phosphorus oxides with respect to S3 can be correlated with a higher probability of black-P lattice deformation. It is not surprising then that the samples with the highest concentration of initial oxides are found to be the most reactive when exposed to identical oxidizing environments. It is interesting to note that during the following half cycle ALD process, there is no detectable phosphorus oxides within the range of 133−136 eV on sample S3, indicating that S3 is essentially phosphorus oxide free. To conﬁrm the reproducibility, a second phosphorus oxide free sample was prepared and analyzed by XPS after atomic layer deposition, the results of which are shown in Figure S3 of the Supporting Information. These results are consistent and indicate that the TMA or water
3. RESULTS AND DISCUSSION Figure 1a compares the deconvolution of P 2p core level XPS spectra from the S1, S2, and S3 samples during the ﬁrst stages of the ALD process. On the initial sample surfaces, the concentration of the oxidized phosphorus species (labeled as POx, e.g., P2O3)23 at 134.2 eV clearly increases with ambient air exposure time: S1 shows the highest oxide concentration, whereas sample S2 is slightly oxidized and the oxidation is
Figure 1. (a) XPS spectra are showing the evolution of P 2p core level from the S1, S2, and S3 samples during the half cycle ALD process. Phosphorus oxide is below the limit of detection on the S3 sample. (b) Integrated intensity ratio of the total phosphorus oxide to that of the bulk black-P peak (IP‑O/IP‑P), up to the initial 5 ALD cycles for the S1, S2, and S3 samples, respectively. B
DOI: 10.1021/acsami.5b03192 ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXX
ACS Applied Materials & Interfaces
oxygen and in fact a detailed analysis of the O 1s spectra (shown in Figure S1 of the Supporting Information), shows that the total concentration of oxygen on the surface is actually higher for S3 than for S2. This strongly suggests that surface adventitious contamination could also enhance the nucleation of Al2O332 and become the dominant mechanism in the case of low POx concentration. Because the growth rates on these samples are diﬀerent, a quantitative comparison of the rate of phosphorus oxidation as a function of ALD cycles (shown in Figure S4 of the Supporting Information) is not as meaningful as considering the reactions as a function of ALD thickness. Figure 2b shows the ratio of IP‑O/IP‑P as a function of Al2O3 thickness. This ratio can be directly correlated to the concentration of thickness of phosphorus oxides. The ratio plateaus for samples S1 and S2 are very similar so that, once the deposited Al2O3 thickness is more than 1 monolayer (∼0.5 nm), the oxidation rate of the black-P surface decreases due to the nonconformal coverage of Al2O3 ﬁlms, which reduces the available interaction area of the black-P substrate with the water precursor. It is noted that the shakeup loss feature of Al 2s, which overlaps with P 2p, discussed in the Supporting Information (Figure S5), has a negligible eﬀect on accurately determining the intensity of the P 2p peak. Figure 3 shows the Al 2p core level XPS spectra from samples S1, S2, and S3 during the ALD process. The trend in
precursor does not react with the black-P surface under vacuum. The main O 1s peak (∼531.5−533 eV) detected from the initial S3 sample (see Figure S1 of the Supporting Information) corresponds to the physisorbed O−C(H) species. This phenomenon is consistent with recent DFT calculations, which show that water adsorption on a bilayer black-P can occur without phosphorus oxidation.14 Favron et al.9 also show that after black-P is exposed to water under vacuum, no degradation of black-P is detected. Based on our experimental ﬁndings, the increased oxides after annealing and the following half cycle ALD process observed on S1 and S2 samples, are mainly related to the presence of the initial phosphorus oxide itself. The growth of Al2O3 on the three samples is quite diﬀerent, as can be seen in Figure 2a, which shows the thickness of Al2O3
Figure 2. (a) Al2O3 thickness during the ALD process for the S1, S2, and S3 samples. (b) Ratio of IP‑O/IP‑P as a function of Al2O3 thickness.
as a function of ALD cycles on all three substrates. The thickness is calculated from the attenuation of the P 2p peak (see the Supporting Information). Focusing ﬁrst on samples S1 and S2, which both started with detectable phosphorus oxide concentrations, it is clear that the growth rate on S1 is signiﬁcantly higher. This can be explained by the higher concentration of nucleation sites aﬀorded by the increased defects and phosphorus oxide concentration. The relatively slow growth rate (